# Characterisation of surface martensite-austenite

date post

22-Jan-2022Category

## Documents

view

0download

0

Embed Size (px)

### Transcript of Characterisation of surface martensite-austenite

Characterisation of surface martensite-austenite transformation during finish turning of an AISI S15500 stainless steelSubmitted on 26 Feb 2017

HAL is a multi-disciplinary open access archive for the deposit and dissemination of sci- entific research documents, whether they are pub- lished or not. The documents may come from teaching and research institutions in France or abroad, or from public or private research centers.

L’archive ouverte pluridisciplinaire HAL, est destinée au dépôt et à la diffusion de documents scientifiques de niveau recherche, publiés ou non, émanant des établissements d’enseignement et de recherche français ou étrangers, des laboratoires publics ou privés.

Distributed under a Creative Commons Attribution| 4.0 International License

Characterisation of surface martensite-austenite transformation during finish turning of an AISI S15500

stainless steel Alexandre Mondelin, Joël Rech, Eric Feulvarch, Michel Coret

To cite this version: Alexandre Mondelin, Joël Rech, Eric Feulvarch, Michel Coret. Characterisation of surface martensite-austenite transformation during finish turning of an AISI S15500 stainless steel. Inter- national Journal of Machining and Machinability of Materials, Inderscience, 2014, 15, pp.101-121. 10.1504/IJMMM.2014.059190. hal-01005923

Characterisation of surface martensite-austenite transformation during finish turning of an AISI S15500 stainless steel

Alexandre Mondelin Université de Lyon, ENISE, LTDS, UMR CNRS 5513, 58 Rue Jean Parot, 42023 Saint-Etienne, France and Université de Lyon, INSA, LaMCoS, UMR CNRS 5259, 27 Avenue Jean Capelle, 69621 Villeurbanne, France E-mail: [email protected]

Joël Rech and Eric Feulvarch Université de Lyon, ENISE, LTDS, UMR CNRS 5513, 58 Rue Jean Parot, 42023 Saint-Etienne, France E-mail: [email protected] E-mail: [email protected]

Michel Coret École Centrale de Nantes, GeM, UMR CNRS 6183, 1 rue de la Noë BP 92101, 44321 Nantes cedex 3, France E-mail: [email protected]

Abstract: During machining, extreme temperature conditions appear in the cutting zone (from 700 to 1,000°C with heating rates around 106 °C/s). Consequently, the metallurgical models used to simulate the impact of the manufacturing process must be adapted to this fast thermal kinetics. Stress-free dilatometry tests have been performed to determine the austenisation kinetics of an AISI S15500 martensitic stainless steel and to identify a phenomenological model. Experimental heating rates vary from 6 °C/s to 11,000 °C/s. The metallurgical model calibrated for high heating rates, has been applied to a typical machining thermal cycle. It has been shown that martensite→austenite transformation does not have the time to significantly occur during the finish turning of AISI S15500 under standard cutting conditions. This result has been confirmed using retained austenite measurements in the machined surface layer.

Keywords: dilatometry; martensite-austenite transformation; high heating rate; turning; metallurgical model; surface integrity.

1 Introduction

Precipitated hardening (PH) stainless steels (like an AISI S15500 steel) show excellent mechanical properties, low distortion, excellent weldability and good corrosion resistance. That is why they are used in the aerospace and nuclear industries. Moreover, predicting the fatigue resistance of mechanical parts is crucial to these industries. Several studies (like Liu and Yang, 2001) have shown that fatigue resistance is directly and significantly influenced by several parameters such as surface roughness (Smith et al., 2007), residual stress (Yang et al., 2002) and microstructure (Bissey-Breton et al., 2007), which are commonly summarised by the term ‘surface integrity’ (Davim, 2008). The influence of surface integrity on the functional performance and lifetime of machined

1

components has been widely discussed in the literature (Jawahir et al., 2011). Surface integrity depends on the thermo-mechanical loadings induced by all previous manufacturing operations, even if the final operation has a major responsibility (Rech et al., 2008). Among the finishing operations applied to critical parts, longitudinal finish turning is widely used. Moreover, the influence of the surface integrity and the effects of microstructure changes on residual stresses in the machined part are really significant and cannot be overlooked (Davim, 2008), especially when the trend is to machine stainless steel using high speed turning (Fernández-Abia et al., 2012).

This strong relationship between surface integrity and fatigue resistance leads to a need for predictive models of microstructure changes and residual stress levels. Currently in the literature, most models only focus on residual stress prediction (Valiorgue et al., 2012). The effects of microstructure changes are not taken into account (Outeiro et al., 2008). On the other hand, some studies try to consider phase transformation during machining in order to predict the final surface integrity (and especially surface layers). Different approaches and models are used. Aramcharoen and Mativenga (2008), who works on hard turning impact on tempered steels, provides a good overview of different studies and explanations for white layer formation. For example, Chou and Song (2005) worked on the surface layer predictions in the finish hard turning of AISI52100 steel (60–62 HRc). An analytical thermal model is used to obtain the final temperature distributions due to the overall heat sources. Chou and Song (2005) assume that the white layer in steel machining is the phase transformation (austenitisation) product. So, the metallurgical model is only based on one phase transformation temperature (727°C, which is the austenitisation transformation temperature of steel in equilibrium conditions). The penetration depth of austenitising temperature is used to estimate the white layer depth. The thermal kinetic influence is not taken into account.

A comparable study on the hard-turning of AISI52100 is presented by Umbrello and Filice (2009). This paper presents an experimental and numerical approach to improve the surface integrity by incorporating the white and dark layer formation. The phase transformation criteria are based on hardness modification and on an austenite-start temperature. The austenite-start temperature ranges from 550°C to 650°C (depending of the initial material hardness but not on the heating rate).

Ramesh and Melkote (2008) suggested using the Clausius-Clayperon equation to account for the effect of pressure (stress) on the austenite start temperature. AISI 52100 steel yields a final α’–γ transformation temperature of 614°C. In the numerical machining model, if the temperature of a material point being analysed exceeds the austenite start temperature, it is assumed to be instantaneously austenitised. Only two austenitisation levels are considered: 0% and 100% of austenite.

This state-of-art survey highlights the difficulty of current studies to calibrate a metallurgical model adapted to the high thermal kinetics of machining. The temporal aspect of the martensite to austenite transformation is often neglected. A simple austenitisation start temperature is often used. This approach is only valid in the equilibrium condition of temperature (or for very low heating rates such as 60°C/hour (Constant et al., 1992). That is clearly not the case during a machining operation. The transitional step of the α’→γ transformation is not considered and models are only able to make predictions if autenitisation occurs or not (two transformation levels).

Martensite to austenite transformation occurs with a diffusional process (Constant et al., 1992). It means a move of carbon atoms along distances higher than the elementary

2

size of the crystal structure. The result is that austenitisation is not instantaneous and very dependent on thermal kinetics (Figure 1, Brosse, 2009). Finally, a metallurgical transformation model used in machining simulation should be able to predict the proportion of initial and produced phases during the machining process. The model should inevitably integrate the thermal kinetics (heating and cooling rates) in the phase proportion calculation.

Figure 1 Evolution of the austenite proportion as a function of the temperature for different heating rates for an AISI5210 steel (see online version for colours)

In Chou (2002)’s study, the effects of machining thermal kinetics are mentioned. Chou (2002) uses an equivalent analytically computed heat source moved on the machined surface to predict the surface hardening of AISI4340 steel. It gives a temporal response of temperature at 13 µm below the surface. The maximum temperature reached is 1,300°C (with a heating rate higher than 5.5 × 106°C/s–1). Indeed Chou (2002) explains that the time interval during which the material was exposed above austenitising temperature (Ac3 of AISI4340 steel is set to 774°C) is only 0.3 ms, far shorter than the time scale in conventional surface hardening. Chou (2002) explains that such short time austenitising is in contradiction with the time-dependence of the autenitisation reaction. Then Chou (2002) suggests that stress/strain significantly contribute to the hardening process.

In other fields than machining, some authors have also tried to work on phase changes using metallurgical model adapted to high thermal kinetics. This is particularly the case for surface hardening treatments. Patwa and Shin (2007) explain the difficulty of considering the formation of austenite in the case of a laser surface heating. Indeed, this time-dependent transformation needs sufficient time for completion or would otherwise be completed only at a higher temperature. In other words, the smaller the time available for diffusion, the higher would be the required maximal reached temperature to obtain a completed austenitisation. Patwa and Shin (2007) describe a kinetic model describing pearlite dissolution and carbon redistribution in austenite to predict surface microstructure and hardness without the need of any experimental data.

3

From a more experimental point of view, Miokovi et al. (2006) and Miokovi et al. (2007) study the surface hardening of AISI4140 steel by laser heating. To calibrate a suitable metallurgical model, Miokovi et al. (2006) performs dilatometry tests with rapid heating (up to 10,000°C/s–1) and cooling (up to 3,000°C/s–1). This work perfectly illustrates the time dependence of the austenitic transformation (variation of the phase change temperatures) and its diffusive nature in the case of AISI4140 steel. Similarly, Reti et al. (1999) explain that the issue is the same during a surface heating by induction. The problem here is that, during a short cycle induction heating of 50 CrMo 4 steel, homogenous austenite may not be obtained. The proportion of transformed phase and so the steel hardness obtained after induction heating and rapid quenching are functions of heating time and final heating temperature. So, Reti et al. (1999) suggests a new phenomenological model and computational method to take into account this kinetic aspect.

Finally, it has been shown that it is important to consider thermal kinetics in an austenitisation model suitable for machining processes. Indeed, this problem of rapid austenitisation, well known in other fields of study for the prediction of phase changes for high thermal kinetics, must also be taken into account for machining. Then two major difficulties arise with this argument.

The first one is directly due to the thermal conditions of the machining process. A great number of studies have shown that metallic fabrication processes, and particularly machining, lead to extremely fast thermal cycles. Poulachon (1999) estimates the heating rate of steel during a hard turning operation to be 2.1 × 106°C/s. The analytical model of Burns et al. (2009) estimate the heating rate to be 1.62 × 106°C/s during orthogonal machining of AISI 1045 steel. Chou and Evans (1999) model estimates the cooling of an AISI52100 steel to be –3.6 × 104°C/s during dry turning whereas Mondelin et al. (2011)’s model quantifies the cooling rate at –106°C/s during the lubricated turning of AISI S15500 . This thermal kinetics is clearly different from cooling rates ordinarily associated with classical quenching operations (from –170°C/s to –1,000°C/s according to Krauss (1990) and Lee and Lee (2008). These very high cooling rates (even during dry machining) are mainly due to the heat conduction from the small cutting zone to the rest of the part.

The second difficulty is related to the nature of the austenitisation reaction itself in superheating conditions. Indeed, extremely high heating rates seem to go against the classical decomposition of martensite into austenite by carbon diffusion (time-dependent nature of diffusional phase transformation). Nevertheless, studies of Leem et al. (2001) and Kappoor and Batra (2004) have shown that the transformation of martensite to austenite can also occur without diffusion using an operation called ‘reverse transformation’. It means that the phase change does not occur with the long-range diffusion of atoms but rather with a form of movement (sliding and shearing) of the atomic planes. In the literature these two types of austenite transformation according to the heating rate have been reported. The debate on the displacive α→γ transformation under high thermal kinetics is still a controversial subject. So, the point is to choose experimental criteria to distinguish these two modes of transformation during rapid heating. The variation of Ac1 and Ac3 (start and end temperature of the austenite transformation) with the heating rate is often considered.

For example, Leem et al. (2001) have studied a martensitic low carbon stainless steel (such as the AISI S15500). According to Leem et al. (2001), below a heating rate of

4

10°C/s the austenite transformation is performed by diffusion. Above 10°C/s, it is performed by a diffusionless shear mechanism (the reverse martensitic transformation). This conclusion is justified by the dependence of Ac1 and Ac3 (start and end temperature of the austenite transformation) on the heating rate below 10°C/s. On the contrary, above 10°C/s, Ac1 and Ac3 become stable. Moreover, Kappoor and Batra (2004) deal with the effects of the heating rate on the austenite transformation kinetics in 17-4PH steel (a martensitic stainless steel close to AISI S15500). Their conclusions show that the austenite transformation is performed by diffusion at low rates and by a shearing process at high rates. Their conclusions are based on the analysis of the activation energy required for austenite formation. Nevertheless, contrary to what happens in Leem et al. (2001)’s study, Ac1 and Ac3 temperatures are not stabilised and keep rising as the heating rate increases. This contradicts Leem et al. (2001)’s study in which the variation of Ac1 and Ac3 with the heating rate demonstrates a diffusion mode of transformation. Constant et al. (1992), basing their assumptions on Orlich et al. (1973)’s study, show curves illustrating the transformation of an AISI4135 steel during rapid heating without a holding temperature. The maximal heating rate is 2,400°C/s which is a very high value in the literature (generally, heating rates used to calibrate metallurgical models are ten times lower, close to 100°C/s). A permanent variation (increase) of Ac1 and Ac3 temperatures has been observed when the heating rate rises. There is no stabilisation of these temperatures [Ac1 and Ac3 stabilisation is considered by Leem et al. (2001) as a consequence of diffusionless transformation].

Studies related to the austenite transformation kinetics of AISI S15500 are very rare. Wu (2007)’s works deal with the characterisation of AISI S15500 phase changes in order to model its welding. Nevertheless, heating rates are limited to 5°C/s. Similarly, Herny et al. (2008) study AISI S15500 heating up to 1,050°C but the results are principally focused on copper precipitation phases and the heating and cooling rates are very low (5°C/min).

With regard to diffusive transformations (like austenitisation), differential formulations are generally used. Leblond and Devaux (1984) phenomenological model is based on a simple law:

− = eqZ Z

(1)

( , ) ( , )

(2)

The influence of the different model parameters (Zeq, τ, Ac1 and Ac3) is illustrated in Figure 2 showing the austenite proportion Zγ as a function of the temperature T for different heating rates ( 1 2 3, ,T T T ). Finally, this form of Leblond’s model is utilised in the

5

rest of this study because of the simplicity of its parameters and its identification, its easy implementation in finite element calculation codes and its good adequacy to model anisothermal diffusive transformations (time-dependent transformations). Various approaches and improvements make it possible to take into account other transformation characteristics (grain size, carbon concentration, …) which will not be developed here.

Figure 2 Influence of Leblond model parameters (see online version for colours)

Experimental resources used to calibrate metallurgical models are multiple in the literature. With regard to heating devices, the Joule effect heating (by induced or direct current) is widely used. The stress-free dilatometry method, used by Leem et al. (2001) and Kappoor and Batra (2004) for example, consists in measuring the deformation of a sample subjected to no stress except for the thermal one (Figure 3). The beginning of the phase transformation is identified by the loss in the linearity of the temperature-deformation curve.

Figure 3 Experimental set-up: positioning the sample in the Gleeble jaws and locations of temperature and dilatation measurements on the stress-free dilatometry sample (see online version for colours)

Moreover, this type of curve permits to obtain the proportion of phase formed during the transformation as shown by Leblond et al. (1986). Indeed, during stress-free dilatometry, the total deformation is equal to the thermal deformation. Moreover the mean thermal

6

( ) ( )( )

' '

' '

k k T To α α γ

γ γ α α γ

ε

ε (3)

where the subscript indicates the averaged phase and 'Δ To α γε is the volumetric density

difference between the α’ phase and the γ phase at temperature To. Thus, the stress-free dilatometry method has been chosen for this study. The

capacities of the thermo-mechanical simulator Gleeble®, coupled with the specific sample shape, permit to reach high heating rates and measure the resulting deformations with great accuracy.

Therefore, a stress-free dilatometry study has been performed for heating rates from 6°C/s to 11,000°C/s. This very wide range allows focusing on Ac1 and Ac3 temperature variations according to thermal kinetics first. So based on these results, the time-dependent nature of the martensite to austenite transformation is revealed over the whole heating rate range. The parameters of Leblond model (Leblond and Devaux, 1984) are calibrated for the thermal kinetics studied. Then the calibrated metallurgical model is combined with a thermal cycle (heating and cooling phase) characteristic of a turning operation. The proportion of austenite formed during this machining operation is then computed.

2 Stress-free dilatometry study

2.1 Experimental set-up

The aim of this stress-free dilatometry study is to deal with phase changes (and in particular the austenisation rate) at very high heating rates. Experiments are carried out to extract two types of information: the variations of Ac1 and Ac3 temperatures and the transformation activation energy according to the heating rate.

The material studied is an AISI S15500 (also known as 15-5PH steel), a martensitic precipitation-hardening stainless steel in H1025 (40 HRC) conditions. The chemical composition of an AISI S15500 steel in wt% is listed in Table 1. Table 1 Chemical composition of AISI S15500 stainless steel in wt%

C Mn Si Cr Ni Cu Nb S P Fe

0.07 Max.

1.0 Max.

1.0 Max.

0.04 Max. Bal.

The capacities of the thermo-mechanical power-controlled simulator Gleeble® were used to reach high heating rates. The heating, produced by Joule effect, depends on the current intensity transmitted and is located in the smallest diameter zone of the sample (Figure 3).

7

Dilatation measurements are performed by means of a radial dilatometer. This method permits to eliminate problems related to important axial temperature gradients. The temperature measurements are performed by means of an 80 µm diameter (type K) thermocouple welded on the measured diameter of the sample.

Each measurement was replicated at least twice. The maximal measurement uncertainty was set to ±20°C for Ac1 and ±35°C for Ac3 for the highest heating rates. This is due to the difficulty to precisely locate the loss in the linearity of the temperature-deformation curve and measurement reproducibility.

Heating is quasi-linear (Figure 4) and lasts from 160 s (up to 960°C at 6°C/s) to 0.1 s (up to 1,100°C at 11,000°C/s). Cooling is free (convection with ambient air and conduction with the clamping jaws). The maximal cooling rate is about –90°C/s when heating stops.

One of the sample extremities is fixed; the other is free to move axially. Nevertheless, constant friction forces on the moving jaw induce residual stresses on the specimen (about 80 N→11 MPa) without any notable effects on dilatometry measurements (Figure 5).

Figure 4 Thermal cycle (a) heating and cooling (b) example of time temperature derivative during heating at 7,500°C/s (see online version for colours)

8

Figure 5 Stress-free dilatometry measurements for…

HAL is a multi-disciplinary open access archive for the deposit and dissemination of sci- entific research documents, whether they are pub- lished or not. The documents may come from teaching and research institutions in France or abroad, or from public or private research centers.

L’archive ouverte pluridisciplinaire HAL, est destinée au dépôt et à la diffusion de documents scientifiques de niveau recherche, publiés ou non, émanant des établissements d’enseignement et de recherche français ou étrangers, des laboratoires publics ou privés.

Distributed under a Creative Commons Attribution| 4.0 International License

Characterisation of surface martensite-austenite transformation during finish turning of an AISI S15500

stainless steel Alexandre Mondelin, Joël Rech, Eric Feulvarch, Michel Coret

To cite this version: Alexandre Mondelin, Joël Rech, Eric Feulvarch, Michel Coret. Characterisation of surface martensite-austenite transformation during finish turning of an AISI S15500 stainless steel. Inter- national Journal of Machining and Machinability of Materials, Inderscience, 2014, 15, pp.101-121. 10.1504/IJMMM.2014.059190. hal-01005923

Characterisation of surface martensite-austenite transformation during finish turning of an AISI S15500 stainless steel

Alexandre Mondelin Université de Lyon, ENISE, LTDS, UMR CNRS 5513, 58 Rue Jean Parot, 42023 Saint-Etienne, France and Université de Lyon, INSA, LaMCoS, UMR CNRS 5259, 27 Avenue Jean Capelle, 69621 Villeurbanne, France E-mail: [email protected]

Joël Rech and Eric Feulvarch Université de Lyon, ENISE, LTDS, UMR CNRS 5513, 58 Rue Jean Parot, 42023 Saint-Etienne, France E-mail: [email protected] E-mail: [email protected]

Michel Coret École Centrale de Nantes, GeM, UMR CNRS 6183, 1 rue de la Noë BP 92101, 44321 Nantes cedex 3, France E-mail: [email protected]

Abstract: During machining, extreme temperature conditions appear in the cutting zone (from 700 to 1,000°C with heating rates around 106 °C/s). Consequently, the metallurgical models used to simulate the impact of the manufacturing process must be adapted to this fast thermal kinetics. Stress-free dilatometry tests have been performed to determine the austenisation kinetics of an AISI S15500 martensitic stainless steel and to identify a phenomenological model. Experimental heating rates vary from 6 °C/s to 11,000 °C/s. The metallurgical model calibrated for high heating rates, has been applied to a typical machining thermal cycle. It has been shown that martensite→austenite transformation does not have the time to significantly occur during the finish turning of AISI S15500 under standard cutting conditions. This result has been confirmed using retained austenite measurements in the machined surface layer.

Keywords: dilatometry; martensite-austenite transformation; high heating rate; turning; metallurgical model; surface integrity.

1 Introduction

Precipitated hardening (PH) stainless steels (like an AISI S15500 steel) show excellent mechanical properties, low distortion, excellent weldability and good corrosion resistance. That is why they are used in the aerospace and nuclear industries. Moreover, predicting the fatigue resistance of mechanical parts is crucial to these industries. Several studies (like Liu and Yang, 2001) have shown that fatigue resistance is directly and significantly influenced by several parameters such as surface roughness (Smith et al., 2007), residual stress (Yang et al., 2002) and microstructure (Bissey-Breton et al., 2007), which are commonly summarised by the term ‘surface integrity’ (Davim, 2008). The influence of surface integrity on the functional performance and lifetime of machined

1

components has been widely discussed in the literature (Jawahir et al., 2011). Surface integrity depends on the thermo-mechanical loadings induced by all previous manufacturing operations, even if the final operation has a major responsibility (Rech et al., 2008). Among the finishing operations applied to critical parts, longitudinal finish turning is widely used. Moreover, the influence of the surface integrity and the effects of microstructure changes on residual stresses in the machined part are really significant and cannot be overlooked (Davim, 2008), especially when the trend is to machine stainless steel using high speed turning (Fernández-Abia et al., 2012).

This strong relationship between surface integrity and fatigue resistance leads to a need for predictive models of microstructure changes and residual stress levels. Currently in the literature, most models only focus on residual stress prediction (Valiorgue et al., 2012). The effects of microstructure changes are not taken into account (Outeiro et al., 2008). On the other hand, some studies try to consider phase transformation during machining in order to predict the final surface integrity (and especially surface layers). Different approaches and models are used. Aramcharoen and Mativenga (2008), who works on hard turning impact on tempered steels, provides a good overview of different studies and explanations for white layer formation. For example, Chou and Song (2005) worked on the surface layer predictions in the finish hard turning of AISI52100 steel (60–62 HRc). An analytical thermal model is used to obtain the final temperature distributions due to the overall heat sources. Chou and Song (2005) assume that the white layer in steel machining is the phase transformation (austenitisation) product. So, the metallurgical model is only based on one phase transformation temperature (727°C, which is the austenitisation transformation temperature of steel in equilibrium conditions). The penetration depth of austenitising temperature is used to estimate the white layer depth. The thermal kinetic influence is not taken into account.

A comparable study on the hard-turning of AISI52100 is presented by Umbrello and Filice (2009). This paper presents an experimental and numerical approach to improve the surface integrity by incorporating the white and dark layer formation. The phase transformation criteria are based on hardness modification and on an austenite-start temperature. The austenite-start temperature ranges from 550°C to 650°C (depending of the initial material hardness but not on the heating rate).

Ramesh and Melkote (2008) suggested using the Clausius-Clayperon equation to account for the effect of pressure (stress) on the austenite start temperature. AISI 52100 steel yields a final α’–γ transformation temperature of 614°C. In the numerical machining model, if the temperature of a material point being analysed exceeds the austenite start temperature, it is assumed to be instantaneously austenitised. Only two austenitisation levels are considered: 0% and 100% of austenite.

This state-of-art survey highlights the difficulty of current studies to calibrate a metallurgical model adapted to the high thermal kinetics of machining. The temporal aspect of the martensite to austenite transformation is often neglected. A simple austenitisation start temperature is often used. This approach is only valid in the equilibrium condition of temperature (or for very low heating rates such as 60°C/hour (Constant et al., 1992). That is clearly not the case during a machining operation. The transitional step of the α’→γ transformation is not considered and models are only able to make predictions if autenitisation occurs or not (two transformation levels).

Martensite to austenite transformation occurs with a diffusional process (Constant et al., 1992). It means a move of carbon atoms along distances higher than the elementary

2

size of the crystal structure. The result is that austenitisation is not instantaneous and very dependent on thermal kinetics (Figure 1, Brosse, 2009). Finally, a metallurgical transformation model used in machining simulation should be able to predict the proportion of initial and produced phases during the machining process. The model should inevitably integrate the thermal kinetics (heating and cooling rates) in the phase proportion calculation.

Figure 1 Evolution of the austenite proportion as a function of the temperature for different heating rates for an AISI5210 steel (see online version for colours)

In Chou (2002)’s study, the effects of machining thermal kinetics are mentioned. Chou (2002) uses an equivalent analytically computed heat source moved on the machined surface to predict the surface hardening of AISI4340 steel. It gives a temporal response of temperature at 13 µm below the surface. The maximum temperature reached is 1,300°C (with a heating rate higher than 5.5 × 106°C/s–1). Indeed Chou (2002) explains that the time interval during which the material was exposed above austenitising temperature (Ac3 of AISI4340 steel is set to 774°C) is only 0.3 ms, far shorter than the time scale in conventional surface hardening. Chou (2002) explains that such short time austenitising is in contradiction with the time-dependence of the autenitisation reaction. Then Chou (2002) suggests that stress/strain significantly contribute to the hardening process.

In other fields than machining, some authors have also tried to work on phase changes using metallurgical model adapted to high thermal kinetics. This is particularly the case for surface hardening treatments. Patwa and Shin (2007) explain the difficulty of considering the formation of austenite in the case of a laser surface heating. Indeed, this time-dependent transformation needs sufficient time for completion or would otherwise be completed only at a higher temperature. In other words, the smaller the time available for diffusion, the higher would be the required maximal reached temperature to obtain a completed austenitisation. Patwa and Shin (2007) describe a kinetic model describing pearlite dissolution and carbon redistribution in austenite to predict surface microstructure and hardness without the need of any experimental data.

3

From a more experimental point of view, Miokovi et al. (2006) and Miokovi et al. (2007) study the surface hardening of AISI4140 steel by laser heating. To calibrate a suitable metallurgical model, Miokovi et al. (2006) performs dilatometry tests with rapid heating (up to 10,000°C/s–1) and cooling (up to 3,000°C/s–1). This work perfectly illustrates the time dependence of the austenitic transformation (variation of the phase change temperatures) and its diffusive nature in the case of AISI4140 steel. Similarly, Reti et al. (1999) explain that the issue is the same during a surface heating by induction. The problem here is that, during a short cycle induction heating of 50 CrMo 4 steel, homogenous austenite may not be obtained. The proportion of transformed phase and so the steel hardness obtained after induction heating and rapid quenching are functions of heating time and final heating temperature. So, Reti et al. (1999) suggests a new phenomenological model and computational method to take into account this kinetic aspect.

Finally, it has been shown that it is important to consider thermal kinetics in an austenitisation model suitable for machining processes. Indeed, this problem of rapid austenitisation, well known in other fields of study for the prediction of phase changes for high thermal kinetics, must also be taken into account for machining. Then two major difficulties arise with this argument.

The first one is directly due to the thermal conditions of the machining process. A great number of studies have shown that metallic fabrication processes, and particularly machining, lead to extremely fast thermal cycles. Poulachon (1999) estimates the heating rate of steel during a hard turning operation to be 2.1 × 106°C/s. The analytical model of Burns et al. (2009) estimate the heating rate to be 1.62 × 106°C/s during orthogonal machining of AISI 1045 steel. Chou and Evans (1999) model estimates the cooling of an AISI52100 steel to be –3.6 × 104°C/s during dry turning whereas Mondelin et al. (2011)’s model quantifies the cooling rate at –106°C/s during the lubricated turning of AISI S15500 . This thermal kinetics is clearly different from cooling rates ordinarily associated with classical quenching operations (from –170°C/s to –1,000°C/s according to Krauss (1990) and Lee and Lee (2008). These very high cooling rates (even during dry machining) are mainly due to the heat conduction from the small cutting zone to the rest of the part.

The second difficulty is related to the nature of the austenitisation reaction itself in superheating conditions. Indeed, extremely high heating rates seem to go against the classical decomposition of martensite into austenite by carbon diffusion (time-dependent nature of diffusional phase transformation). Nevertheless, studies of Leem et al. (2001) and Kappoor and Batra (2004) have shown that the transformation of martensite to austenite can also occur without diffusion using an operation called ‘reverse transformation’. It means that the phase change does not occur with the long-range diffusion of atoms but rather with a form of movement (sliding and shearing) of the atomic planes. In the literature these two types of austenite transformation according to the heating rate have been reported. The debate on the displacive α→γ transformation under high thermal kinetics is still a controversial subject. So, the point is to choose experimental criteria to distinguish these two modes of transformation during rapid heating. The variation of Ac1 and Ac3 (start and end temperature of the austenite transformation) with the heating rate is often considered.

For example, Leem et al. (2001) have studied a martensitic low carbon stainless steel (such as the AISI S15500). According to Leem et al. (2001), below a heating rate of

4

10°C/s the austenite transformation is performed by diffusion. Above 10°C/s, it is performed by a diffusionless shear mechanism (the reverse martensitic transformation). This conclusion is justified by the dependence of Ac1 and Ac3 (start and end temperature of the austenite transformation) on the heating rate below 10°C/s. On the contrary, above 10°C/s, Ac1 and Ac3 become stable. Moreover, Kappoor and Batra (2004) deal with the effects of the heating rate on the austenite transformation kinetics in 17-4PH steel (a martensitic stainless steel close to AISI S15500). Their conclusions show that the austenite transformation is performed by diffusion at low rates and by a shearing process at high rates. Their conclusions are based on the analysis of the activation energy required for austenite formation. Nevertheless, contrary to what happens in Leem et al. (2001)’s study, Ac1 and Ac3 temperatures are not stabilised and keep rising as the heating rate increases. This contradicts Leem et al. (2001)’s study in which the variation of Ac1 and Ac3 with the heating rate demonstrates a diffusion mode of transformation. Constant et al. (1992), basing their assumptions on Orlich et al. (1973)’s study, show curves illustrating the transformation of an AISI4135 steel during rapid heating without a holding temperature. The maximal heating rate is 2,400°C/s which is a very high value in the literature (generally, heating rates used to calibrate metallurgical models are ten times lower, close to 100°C/s). A permanent variation (increase) of Ac1 and Ac3 temperatures has been observed when the heating rate rises. There is no stabilisation of these temperatures [Ac1 and Ac3 stabilisation is considered by Leem et al. (2001) as a consequence of diffusionless transformation].

Studies related to the austenite transformation kinetics of AISI S15500 are very rare. Wu (2007)’s works deal with the characterisation of AISI S15500 phase changes in order to model its welding. Nevertheless, heating rates are limited to 5°C/s. Similarly, Herny et al. (2008) study AISI S15500 heating up to 1,050°C but the results are principally focused on copper precipitation phases and the heating and cooling rates are very low (5°C/min).

With regard to diffusive transformations (like austenitisation), differential formulations are generally used. Leblond and Devaux (1984) phenomenological model is based on a simple law:

− = eqZ Z

(1)

( , ) ( , )

(2)

The influence of the different model parameters (Zeq, τ, Ac1 and Ac3) is illustrated in Figure 2 showing the austenite proportion Zγ as a function of the temperature T for different heating rates ( 1 2 3, ,T T T ). Finally, this form of Leblond’s model is utilised in the

5

rest of this study because of the simplicity of its parameters and its identification, its easy implementation in finite element calculation codes and its good adequacy to model anisothermal diffusive transformations (time-dependent transformations). Various approaches and improvements make it possible to take into account other transformation characteristics (grain size, carbon concentration, …) which will not be developed here.

Figure 2 Influence of Leblond model parameters (see online version for colours)

Experimental resources used to calibrate metallurgical models are multiple in the literature. With regard to heating devices, the Joule effect heating (by induced or direct current) is widely used. The stress-free dilatometry method, used by Leem et al. (2001) and Kappoor and Batra (2004) for example, consists in measuring the deformation of a sample subjected to no stress except for the thermal one (Figure 3). The beginning of the phase transformation is identified by the loss in the linearity of the temperature-deformation curve.

Figure 3 Experimental set-up: positioning the sample in the Gleeble jaws and locations of temperature and dilatation measurements on the stress-free dilatometry sample (see online version for colours)

Moreover, this type of curve permits to obtain the proportion of phase formed during the transformation as shown by Leblond et al. (1986). Indeed, during stress-free dilatometry, the total deformation is equal to the thermal deformation. Moreover the mean thermal

6

( ) ( )( )

' '

' '

k k T To α α γ

γ γ α α γ

ε

ε (3)

where the subscript indicates the averaged phase and 'Δ To α γε is the volumetric density

difference between the α’ phase and the γ phase at temperature To. Thus, the stress-free dilatometry method has been chosen for this study. The

capacities of the thermo-mechanical simulator Gleeble®, coupled with the specific sample shape, permit to reach high heating rates and measure the resulting deformations with great accuracy.

Therefore, a stress-free dilatometry study has been performed for heating rates from 6°C/s to 11,000°C/s. This very wide range allows focusing on Ac1 and Ac3 temperature variations according to thermal kinetics first. So based on these results, the time-dependent nature of the martensite to austenite transformation is revealed over the whole heating rate range. The parameters of Leblond model (Leblond and Devaux, 1984) are calibrated for the thermal kinetics studied. Then the calibrated metallurgical model is combined with a thermal cycle (heating and cooling phase) characteristic of a turning operation. The proportion of austenite formed during this machining operation is then computed.

2 Stress-free dilatometry study

2.1 Experimental set-up

The aim of this stress-free dilatometry study is to deal with phase changes (and in particular the austenisation rate) at very high heating rates. Experiments are carried out to extract two types of information: the variations of Ac1 and Ac3 temperatures and the transformation activation energy according to the heating rate.

The material studied is an AISI S15500 (also known as 15-5PH steel), a martensitic precipitation-hardening stainless steel in H1025 (40 HRC) conditions. The chemical composition of an AISI S15500 steel in wt% is listed in Table 1. Table 1 Chemical composition of AISI S15500 stainless steel in wt%

C Mn Si Cr Ni Cu Nb S P Fe

0.07 Max.

1.0 Max.

1.0 Max.

0.04 Max. Bal.

The capacities of the thermo-mechanical power-controlled simulator Gleeble® were used to reach high heating rates. The heating, produced by Joule effect, depends on the current intensity transmitted and is located in the smallest diameter zone of the sample (Figure 3).

7

Dilatation measurements are performed by means of a radial dilatometer. This method permits to eliminate problems related to important axial temperature gradients. The temperature measurements are performed by means of an 80 µm diameter (type K) thermocouple welded on the measured diameter of the sample.

Each measurement was replicated at least twice. The maximal measurement uncertainty was set to ±20°C for Ac1 and ±35°C for Ac3 for the highest heating rates. This is due to the difficulty to precisely locate the loss in the linearity of the temperature-deformation curve and measurement reproducibility.

Heating is quasi-linear (Figure 4) and lasts from 160 s (up to 960°C at 6°C/s) to 0.1 s (up to 1,100°C at 11,000°C/s). Cooling is free (convection with ambient air and conduction with the clamping jaws). The maximal cooling rate is about –90°C/s when heating stops.

One of the sample extremities is fixed; the other is free to move axially. Nevertheless, constant friction forces on the moving jaw induce residual stresses on the specimen (about 80 N→11 MPa) without any notable effects on dilatometry measurements (Figure 5).

Figure 4 Thermal cycle (a) heating and cooling (b) example of time temperature derivative during heating at 7,500°C/s (see online version for colours)

8

Figure 5 Stress-free dilatometry measurements for…